C. R. Physique 3 (2002) 915922Physique applique/Applied physics
DU COMBUSTIBLE NUCLAIRE AUX DCHETS : RECHERCHESACTUELLES
FROM NUCLEAR FUELS TO WASTE: CURRENT RESEARCH
Metallic structural materials in the nuclearenvironment: some problems illustrating new methodsYves BrchetL.T.P.C.M., Institut national polytechnique de Grenoble, domaine universitaire, BP 75, 38402 Saint MartindHeres cedex, France
Received 28 April 2002; accepted after revision 24 June 2002Note presented by douard Brzin.
Abstract The structural components of the nuclear industry are submitted to a number of aggressions,mechanical, chemical and physical (irradiation). As a consequence, the problem ofdurability and ageing of such structures is a key issue. The understanding of the phenomenainvolved implies the description and modelling of atomic scale events (irradiation pointdefects) resulting in fluxes of matter (diffusion under irradiation), in the dynamicevolution of structural defects (dislocation loops, cavities, . . .), with major consequenceson mechanical properties (yield stress, fracture behaviour), with, in addition, phenomenacoupled between mechanical behaviour and chemical environment. It is therefore thetotality of materials science which is involved in understanding the behaviour of metallicstructural materials in the nuclear environment. The aim of the present paper is to illustratesome examples currently under investigation, and some of the new approaches involvedin the understanding of mechanical behaviour (a scale transition from the atomic to themacroscopic). The input from large computer simulations as well as the value of simpleback of the envelope calculations, plus the need for cautious experimental studies will beillustrated. The theme of the ageing of materials, central to this paper, finds applications inmany industrial situations. To cite this article: Y. Brchet, C. R. Physique 3 (2002) 915922. 2002 Acadmie des sciences/ditions scientifiques et mdicales Elsevier SASmetallurgy / defects / irradiation / mechanical properties
Matriaux de structure mtalliques dans le nuclaire : quelquesproblmes, quelques nouvelles mthodes
Rsum Les composants structuraux de lindustrie nuclaire sont soumis des sollicitations mca-niques, chimiques et physiques trs agressives. En consquence le problme de la durabilitet du vieillissement de ces composants est dune importance majeure. La comprhensionde ces phnomnes fait intervenir des mcanismes lchelle atomique (dfauts dirra-diation), des flux de matire (diffusion et diffusion sous irradiation), le dveloppement dedfauts structuraux (boucles de dislocations, cavits), avec des consquences importantessur les comportements mcaniques (limite dlasticit et comportement rupture) et descouplages entre la mcanique et lenvironnement. Cest donc lensemble de la science desmatriaux qui est implique dans la comprhension et la modlisation de ces comporte-
E-mail address: Yves.Brechet@ltpcm.inpg.fr (Y. Brchet). 2002 Acadmie des sciences/ditions scientifiques et mdicales Elsevier SAS. Tous droits rservsS1631-0705(02)01383-X/FLA 915
Y. Brchet / C. R. Physique 3 (2002) 915922
ments. On se propose de brosser un tableau de quelques questions actuellement ltude,du point de vue des changements dchelle (de latomique au macroscopique). Lapport dessimulations numriques aussi bien que les vertus de simples calculs de dos denveloppe ,et la ncessit dtudes exprimentales soignes seront au centre de cet expos. La pro-blmatique du vieillissement des structures ainsi prsente est importante bien au del dudomaine nuclaire et les recherches menes dans ce cadre peuvent trouver des applicationsdans de multiples domaines industriels. Pour citer cet article : Y. Brchet, C. R. Physique3 (2002) 915922. 2002 Acadmie des sciences/ditions scientifiques et mdicales Elsevier SASmtallurgie / dfauts / irradiation / proprits mcaniques
Metallic structural materials in the nuclear industry, and especially the steels used in the main componentsapart from the very core of a nuclear reactor, present a number of specific features which have motivated,in the last decades, numerous research programs. The initial driving force for the studies of materialsbehaviour under irradiation was to build nuclear power plants in the first place . However, with theincreasing age of the production units, and the problem of waste management, the key concept has becomethe ageing of materials under irradiation [2,3].
The environment under which structural materials are operating is very aggressive: it is aggressivein terms of temperature (leading to creep, to precipitation evolution), in terms of chemical interactions(corrosion, oxidation), and in terms of irradiation damage. Operating a nuclear power plant safely requires,in principle, a proper understanding of the properties evolution with time, just like designing a safe turbinereactor for an airplane requires a good evaluation of the damage due to oxidation or creep. In case of doubt,the lazy way to ensure security is the safety factor which amounts to overdimensioning the structures,or to replace the components earlier than really needed. For airplanes, the trend toward weight saving hasmore and more disqualified the use of comfortable safety factors. For nuclear power plants, the need tominimize the amount of radioactive waste leads to the same tendency: more and more it will be necessaryto account for the time evolution of properties with a sufficient accuracy, and that cannot be done by purelyempirical knowledge. A deep understanding of the underlying mechanisms is required in order to derivereliable constitutive laws able to predict materials behaviour for durations much longer that the durationof standard experiments. The aim of this paper is to present some recent developments in this direction, andthe conceptual tools needed for a safe operation of nuclear power plants in the long term.
2. Basic steps for the understanding of the mechanical behaviour of metallic alloys in a nuclearenvironment
A number of phenomena specific to irradiation damage with matter are now well identified .Irradiation is known to shatter the very basic features of matter: it can destroy the crystalline order, itcan introduce structural point defects whose migration will lead to mass fluxes and possible segregation ofchemical species, it can even change the chemical composition of an alloy through atomic transmutation.The variety of metallurgical phenomena which may occur under irradiation and lead to a microstructuralevolution is far beyond the scope of the present paper (for a review, see for instance [7,11]). It will beenough for us to remember that the basic phenomena occurring under irradiation take place at the atomicscale (a few Angstrms).
These microstructural events at the atomic level have consequences at the level of the substructure ofthe material: the state of precipitation can evolve (accelerated coarsening or dissolution of precipitates,appearance of out-of-equilibrium phases), the initial dislocation substructure may be thoroughly modified(creation of dislocation loops, evaporation of the dislocation network, . . .), inner cavities (voids or gas
To cite this article: Y. Brchet, C. R. Physique 3 (2002) 915922
bubbles) may appear. These evolutions take place in the range of scales between 10 nm to 10 m, andthis evolution in the mesostructure is crucial to the understanding of the consequences of irradiation on theplastic behaviour of metallic alloys.
The dislocations responsible for the ability to deform plastically (they are the carriers of plasticity justas electrons in metals are the carriers for electricity) will interact strongly with this mesostructure. Thedefects created will impede their movement, therefore the ability to deform plastically will decrease, andone expects qualitatively that the alloys will become harder and more brittle.
Assuming we understand this modification of the behaviour of dislocations due to the presence of thismicrostructure, our problem is far from being solved. The macroscopic plastic behaviour of the sample is aconsequence of the collective behaviour of dislocations interacting with a population of irradiation defects.Therefore a key issue is on one hand to understand the collective behaviour of the dislocation population,and on the other hand to understand the collective behaviour of irradiation defects leading to the formationof the mesostructure.
Once these two problems are solved, we can hope to understand the mechanical behaviour of a grain ofalloy. A sample on which mechanical tests are performed is never a single grain: it is a polycrystal formedby a collection of grains loosely packed along grain boundaries. Since metals are crystalline, their plasticbehaviour depends on the respective orientation of the crystal reference frame and of the loading directions.The different grains will deform differently and thus the overall behaviour will depend not only on thebehaviour of each grain, but also on their interactions.
Then we come to the understanding of the behaviour of a real sample, at the millimetre scale. However,the story is not over . . . . A real component in a nuclear power plant has a complex geometry, loadings interms of temperature and stress fields are not homogeneous. Possible fracture of the component depends onthe presence of defects in the materials and is thus probabilistic in nature. In the previous steps, physicalmetallurgy was the discipline in charge, now mechanics has to take over. The local approach to failuredeveloped in the French school of fracture mechanics has provided a powerful tool for the transition fromthe local behaviour of the material to the macroscopic behaviour of the component.
The key issues specific to metallic materials in a nuclear environment are the transition from themechanisms occurring at the atomic level (the very cause of irradiation damage) to the materials behaviourat the scale of the grains. The problems posed by the transition from the grain behaviour to the componentare far from being all solved, but they are not specific to nuclear mechanical metallurgy (for a recent reviewof the question, see ). In the next section, we will illustrate by an example the conceptual tools availablefor the understanding of irradiation effect on plastic behaviour.
3. An example of scale transition from the atomic level to grain behaviour: Irradiation hardening
Fig. 1 shows strain curves of a 316 stainless steel after irradiation at 20 C. The main effects are a verylarge increase of the yield stress (multiplied by 2.5), a decrease in the ductility (divided by a factor 4) anda pronounced softening which is very likely to lead to a very damageable strain localisation.
The alloy 316 is a complex material. In order to understand the mechanisms, it is necessary to studymodel materials. The different steps in the understanding reflect the scale transition outlined in theprevious section.
Irradiation damage takes place at the atomistic level, and the atoms are removed from their sites onthe crystalline lattice. The mechanisms are collective effects, and the modelling tool adapted to thisproblem is Molecular Dynamics (MD) [9,10]. It allows, for a given input energy, to predict the amountof free vacancies and interstitial created. It also identifies more complex defects resulting from theinteractions between the point defects. The key step here is to have a reliable interatomic potential,and the progress of ab-initio methods in recent years are now on the way of providing such potentials,both for pure materials and for simple binary alloys.
Y. Brchet / C. R. Physique 3 (2002) 915922
Figure 1. Stress strain curve of an irradiated StainlessSteel with different doses (expressed in dpa,
displacement per atom) (courtesy of C. Pokor,P. Dubuisson, J.P. Massoud).
The point defects created by irradiation are mobile (diffusion) and they interact between them, and withthe other structural defects (dislocations, grain boundaries, . . .). They tend to coalesce into dislocationloops which become strong obstacles to the motion of other dislocations. Modelling this phenomenonis done using cluster dynamics : a population of interstitial or vacancy loops (a cluster of ndefects) evolves by absorbing or rejection a point defect. The master equation ruling this system (takinginto account the bias of each cluster for each type of point defects) is solved either discretely, or usingthe continuous version, or the Fokker Planck equation. This model allows one to predict the size anddensities of loops for a given irradiation dose and a given irradiation temperature. The comparisonbetween predicted quantities and TEM observations on irradiated materials allows one to identifythe adjustable parameters of the model (whose magnitudes are known from physical arguments) andto test its predictive ability. A key issue here is to have the experimental observations allowing forthis comparison: this requires irradiation reactors and special TEM equipment which are crucial to aserious study on irradiation effects.
When the microstructure resulting from irradiation point defect interaction is well described, thepinning efficiency for other moving dislocations has to be investigated . When the Frank loops arelarge enough (more than 10 nm) the classical elasticity theory of dislocation-dislocation interactionis sufficient: it allows one to calculate the pinning strength of the defect, and the theory of collectivepinning of a dislocation by obstacles, well developed for precipitation hardening, applies directly,allowing to predict the evolution of the yield stress as a function of the loop population. When theloops are much smaller, of the order of the dissociation width of the dislocations (1 nm), elastic theoryis dubious, and again the Molecular Dynamics technique is well suited : it allows one to calculatethe pinning strength of the obstacle, but also to show its mobility; the effect of irradiation defects isnot only to pin the dislocations, but also to make their motion more sluggish. The moving defects canalso be annihilated by the moving dislocation. An additional subtlety is the possibility of defaulting theFrank loop, and to decrease the pinning strength of this obstacle that way. From these two mechanisms,it appears that the pinning efficiency of a population of irradiation defects decreases while deformationproceeds: this is the physical origin of the strain softening observed experimentally in Fig. 1.
However, experimentally, it is observed that the strain softening effect appears only when theirradiation dose exceeds a threshold. This comes from the competing effect of work hardening
Pour citer cet article : Y. Brchet, C. R. Physique 3 (2002) 915922
(a strained material hardens due to dislocation interactions) and the sweeping out of irradiation defects.In order to quantify this effect, it is necessary to couple the clas...